Thermoforming - PCToday · PDF file quarterly ® thermoforming. a journal of the...
Embed Size (px)
Transcript of Thermoforming - PCToday · PDF file quarterly ® thermoforming. a journal of the...
A JOURNAL OF THE THERMOFORMING DIVISION OF THE SOCIETY OF PLASTICS ENGINEERS THIRDQUARTER2015nVOLUME34nNUMBER3
NSIDEIThermoformed Packaging 2015 pages 8-9
Improvements in Color Technology pages 28-29
2015 Thermoformer of the Year page 30
2015 Conference Preview pages 38-42
Forming Insights with Data
20 THERMOFORMING QUARTERLY
Comparison Between Thermoforming Tooling Materials Aluminum and HYVAC-LCMByBryanT.Robinson,PennsylvaniaCollegeofTechnology,Williamsport,PA
the tool is syntactic foam while the inner core is constructed of composite spheres. Syntactic foam gets its name from the ordered structure of the spheres (syntactic) and the cellular structure of the material (foam).
Syntactic foam contains preformed hollow spheres that are held together in a binder. The binder typically is an epoxy, urethane, thermoplastic, glass, ceramic or metal. The hollow spheres can be made of thermoplastic, ceramic, or glass. Glass spheres held together with an epoxy binder are the most commonly found in syntactic foam. Figure 1 is a cross-section of the material zoomed in 100 times to allow for a view of the hollow areas (the hollow spheres) and the material around them (the binder.)
Figure 1: Syntactic Foam
Five different types of polymer sheet were used: High Impact Polystyrene (HIPS) 0.080 thick; Polyethylene Terephthalate glycol-modified (PETG) 0.080 thick; KYDEX T (Acrylic PVC) 0.125 thick; Acrylonitrile Butadiene Styrene (ABS) 0.125 thick; and High Density Polyethylene (HDPE) 0.093 thick.
Machine Set-upThe physical set-up of the machine was the same for both molds used in this study. All timers and delays were the same except for the forming time. Changes to the forming time were necessary to meet the part ejection temperature ranges recommended by the manufacturers of each polymer tested. A common oven heating profile was used to eliminate variables, show in Figure 2. The oven on the MAAC Thermoformer has 56 heating zones, 30 quartz heaters on top and 26 glassed-faced ceramic heaters on the bottom. The vacuum box for the HYVAC-LCM was built to match the vacuum box for the aluminum mold to eliminate
AbstractCMT Materials, Inc. hypothesizes that the heavy-gauge vacuum- and pressure-forming industry lacks an effective and affordable mold material that can be used on small-to-medium sized runs. (For the purposes of this paper, small-to-medium is defined as >500 parts and
THERMOFORMING QUARTERLY 21
any variation and for ease of set-up. While processing, the goal was to maintain at least 25in/Hg vacuum. The change over time between molds was 5-10 minutes total. Speed of the change-over minimized oven temperature spikes. All settings remained the same except for the encoders (platen travel) as the vacuum box heights were slightly different.
Figure 2: Oven Profile
The polymer sheets were all cut with matching orientation to a size of 10 x 18.5. For example, all the orientation in the HIPS sheet prior to forming is the same for each the HYVAC-LCM and aluminum tool; the same approach was used for the other four polymer sheets used in this experiment. Consistent orientation eliminated the possibility of shrinkage or material distribution variation between the two molds.
Tool DurabilityIn order to test the durability of the syntactic foam, a small part was made into a saucer about 7 inches in diameter and one half-inch thick. This part was gelled and cured. After curing and annealing the part back down to match the mold characteristics, the sample piece was dropped from 4 feet and did not crack or dent. Further tests would be to drop the HYVAC-LCM and observe the results.
Tool CostThe aluminum tool (donated to PCT by Bayer MaterialScience) was machined from 6061 aluminum that is easily polished for processing clear polymers. The estimated cost for this mold is $2500. The estimated cost to produce a duplicate mold using HYVAC-LCM is calculated using the material cost and the labor necessary to make the tool. The actual raw material cost came to $51.10: $31.54 for the putty and $19.56 for the beads, resin and hardener. This product will eventually be sold in kit form, and the total cost will depend on the size of the mold being built. The necessary labor time is about 10 hours at a rate of $50 per hour. For our purposes, the total cost for the tool ran approximately
$550. In this evaluation, a negative cavity was available and was used to create the mold. No cost was calculated for making a negative cavity. HYVAC-LCM can be machined to shape as a built-up mold or packed in to a negative cavity with no machining required.
Tool ConstructionThe following tool construction is based on building a tool for a front-load washing machine door. This door was used to further study building techniques and a glass door was used so voids could be seen in the syntactic foam lay- up process. Tool construction required two, eight-hour days to complete. The first step was to wax the mold and lay the putty (syntactic foam) along the walls in a 0.5-thick wall. Next, a batch of beads was mixed and coated in an epoxy with catalyst to attach all the beads together so they could be packed into the mold (about 2 hours.) The mold was placed in a 170 degree Fahrenheit oven and gelled overnight. The mold was then slowly cooled to room temperature by lowering the heat in the oven and allowing the part to anneal (about 12 hours of heat and 4 hours to reach room temperature.) After reaching room temperature the voids in the mold surface were filled with the putty again (about one hour) and the mold was placed back in the oven to gel again (12 hours to heat, approximately 4 hours to cool.) Sanding then took place to eliminate all the spots that were filled (about 3 hours). After sanding was complete, the mold was put back in the oven for a final cure at 280 degrees Fahrenheit for 6 hours. The heat was then turned off to allow the mold to anneal back at room temperature (about 6 hours of heating and 4 hours to anneal.) Next the inserts were interpolated by first drilling holes and vacuuming all loose debris out of the area. Some of the holes were filled with Gorilla Glue. The shell of the metal inserts were also coated with Gorilla Glue and the inserts were then placed in the holes (about one hour) allowing the glue to cure and expand. The glued areas were then retouched to fill any extra gaps. Once the glue dried the mold was mounted to a mounting plate with specific holes cut out under the tool to allow vacuum to travel into the beads. It is estimated that it would take about 3 days to create this tool.
Tool WeightThe tool weight is very significant, as the HYVAC-LCM is much lighter and easier to handle than the aluminum tool. The HYVAC-LCM mold and mounting plate weigh only 3.5 pounds. The tool, vacuum box and mounting fixtures combined weigh only 21.5 pounds. The aluminum tool weight including the vacuum box is 38.5 pounds a total difference of 17 pounds (44% more). The use of a lighter tool has a great possibility to reduce machine wear and allow for machine sustainability. The lighter tool will also increase the safety of workers involved with machine set-up.
Forming Cycle TimeThe forming cycle differs from polymer to polymer due to differences in starting material thickness and ejection temperatures. Samples produced from the HYVAC-LCM were formed using two cooling cycles to document the rate of change in temperature over a 10-cycle run and to achieve the ejection temperature suggested by the manufacturer. Using High Impact
22 THERMOFORMING QUARTERLY
Polystyrene (HIPS) as an example, the forming (cooling) time for the HYVAC-LCM was set for 40 and 80 seconds. For the aluminum tool, the forming (cooling) time was set at 60 seconds. The same approach was taken with the other polymers with forming times and ejection temperatures.
Tool TemperatureThe tool temperature was measured before and after forming. The data of importance is that of after forming to see how hot the tool became. As mentioned above, samples were processed in sets of ten, documenting the rise in temperature. The data shown in Figure 3 represents mold temperatures (when processing HIPS material) after forming each of the ten samples, both with a 40 and 80 second forming (cooling) cycle. Temperatures were taken at two points on the tool, illustrated in Figure 4. The tool was measured immediately upon the ejection cycle. The LCM mold can only be cooled by heat dissipation due to its low thermal conductivity. Syntactic foam is approximately 50% air by volume which virtually eliminates thermal conductivity to prevent the sheet from instantly freezing upon contact with the mold. Initial tests showed the mold maintaining a stable temperature after a few shots. In the event the mold continues to rise in temperature, it is possible to regulate the temperature by use of external cooling fans.
Figure 3: Mold Temperature After Forming of HIPS
Figure 4: Aluminum Tool showing points A and B
Material Thickness ProfileMaterial distribution is a main contributor to the overall efficiency of using HYVAC-LCM. When comparing the average
thickness by position for each type of polymer, illustrated in figure 5, the HYVAC-LCM had a more uniform wall thickness. HYVAC-LCM allows the polymer to slide over the tool instead of freezing and stretching as observed on samples produced from the aluminum mold. In addition, it appears that the HYVAC- LCM allowed for distributing material from the perimeter flange or skeleton of the part, resulting in improved material distribution. Figures 6 and 7 show the different m